RESEARCH AND EDUCATION
Fracture resistance of compromised endodontically treated teeth restored with bonded post and cores: An in vitro study Georgios Maroulakos, DDS, MS,a William W. Nagy, DDS,b and Elias D. Kontogiorgos, DDS, PhDc Caries and trauma result in the ABSTRACT loss of coronal tooth structure. Statement of problem. It is unclear which post and core system performs best when bonded to If the loss is substantial, the severely compromised endodontically treated teeth. natural tooth structure cannot Purpose. The purpose of this study was to investigate the fracture resistance and mode of failure of support a restoration, and a severely compromised teeth restored with 3 different adhesively bonded post and core systems. post is necessary to retain an Material and methods. Thirty extracted endodontically treated maxillary anterior teeth were artiﬁcial core that will restore randomly divided into 3 groups, CPC, gold cast post and core; TPC, titanium prefabricated post/ the lost tooth structure. Recomposite resin core; and FPC, quartz ﬁber reinforced post/composite resin core. All posts were maining tooth structure is the adhesively cemented. All cores resembled a central incisor preparation with no remaining tooth most important factor for the structure above the ﬁnish line. Cast gold crowns were fabricated and cemented adhesively. The long-term success of an endspecimens were aged with thermocycling and cyclic loading. Two specimens per group were odontically treated tooth, irrerandomly selected for micro-computed tomographic imaging before and after aging. Failure was induced with a universal testing machine. The mode of failure was characterized by the interface spective of post type1 or post separation. Data were analyzed with 1-way ANOVA (a=.05) followed by post hoc tests (Bonferroni). length.2 However, the real challenge is restoring endResults. A statistically signiﬁcant difference was found among the 3 groups (P=.002). CPC was odontically treated teeth with signiﬁcantly different than TPC (P=.008) or FPC (P=.003). The primary mode of failure for CPC and TPC was root fracture, and for FPC post debonding. inadequate remaining tooth structure.3 Procedures to adConclusions. Severely compromised endodontically treated teeth restored with bonded gold cast dress the lack of remaining post and cores showed signiﬁcantly higher fracture resistance. (J Prosthet Dent 2015;-:---) structure include orthodontic extrusion and surgical crown lengthening. However, they The role of the post is limited when more than 2 mm may compromise the crown/root ratio, resulting in of tooth structure remain.9,10 Other critical factors may be 4 reduced static load failure of the teeth or unfavorable the circumferential presence of tooth structure,11 its esthetic outcomes. location,12 the ferrule width, remaining wall parallelism, A ferrule is “a metal band or ring used to ﬁt the root the resin cement, and the post and core system used.13 5 or crown of a tooth.” It enhances the integrity of the Many different post and core systems are currently endodontically treated tooth by counteracting functional available and differ depending on the post type, design, lever forces, the wedging effect of tapered posts, and surface texture, ﬁt, and material. Studies that compare lateral forces during post insertion.6 A minimum of 1 to various post types have yielded controversial results favoring cast,14-16 ﬁber reinforced,17-21 titanium,20 stain2 mm of remaining tooth structure coronal to the ﬁn6-8 ishing line is necessary to create an adequate ferrule. less steel posts,22 or no speciﬁc type.22,23 Some did not
Supported by the Baylor College of Dentistry Graduate Research Fund. Part of this study was presented as an oral presentation at the 41st Annual Meeting of the American Academy of Dental Research, March 2012, Tampa, Fla. a Assistant Professor, Department of General Dental Sciences, Marquette University School of Dentistry, Milwaukee, Wis. b Professor and Director, Graduate Prosthodontics, Department of Restorative Sciences, Texas A&M University, Baylor College of Dentistry, Dallas, Texas. c Associate Professor, Department of Restorative Sciences, Texas A&M University, Baylor College of Dentistry, Dallas, Texas.
THE JOURNAL OF PROSTHETIC DENTISTRY
Clinical Implications The use of bonded gold cast post and cores could increase the fracture resistance of structurally compromised endodontically treated teeth.
standardize the cement used, and so the systems could not be directly compared.16,21 Resin cements exhibit a higher number of cycles to preliminary failure24 and better retention,25 and they appear to be the most suitable for the cementation of ﬁber posts.25-34 They are also used to cement metal posts and can be used with metal primers that enhance the bond to composite resins.35 Resin cements ﬁnd application in the monoblock theory, in which dentin, post, and core function as a cohesive unit.14,36 The oral cavity is not a static environment. Restorative materials are subjected to dynamic temperature and loading conditions. Simulating those conditions in vitro is essential.37-40 Endodontically treated teeth that cannot provide an adequate ferrule are the most challenging, and the selection of the right type of post may be an important success factor. No studies have compared bonded custom cast post and cores, titanium prefabricated posts/composite resin core, and quartz ﬁber posts/composite resin core in structurally compromised teeth in a simulated oral environment. The results may help to solve the dilemma of post selection in those situations. The purpose of this in vitro study were to compare the fracture resistance of compromised endodontically treated teeth restored with 3 post and core systems and to characterize the types of failure in different groups. The null hypothesis was that no signiﬁcant differences would be found among the 3 groups. MATERIAL AND METHODS Thirty freshly extracted human anterior maxillary teeth (central incisors, lateral incisors, canines) were obtained from patients of Texas A&M University, Baylor College of Dentistry. Written consent was obtained in accordance with the institutional review board. The teeth were cleaned, disinfected (ProSpray C-60; Certol Intl), inspected under light magniﬁcation (Stemi DV4 8.0x; Carl Zeiss MicroImaging, Inc), and radiographed to ensure they were free of cracks or internal resorption. All teeth were sectioned leaving 15 mm of sound tooth structure above the root apex and endodontically treated by using the crown down technique41 with rotary NiTi instrumentation (EndoSequence; Brasseler) until apical instrumentation of ISO 40 and 5.25% sodium hypochlorite irrigation. The taper was 4% after chemomechanical preparation of the root canals. The canals THE JOURNAL OF PROSTHETIC DENTISTRY
Figure 1. Photograph of 3 different post systems tested. CPC, Parapost XP-Lab (plastic pattern for custom cast post and core); TPC, Parapost XH (prefabricated titanium post); FPC, D.T. Light-Post (prefabricated quartz ﬁber post).
were obturated with gutta-percha cones (Dentsply Intl) with warm vertical compaction (sealer, AH Plus; Dentsply Intl). The cones were heat seared (System B; SymbronEndo) and compacted, leaving 4 mm of apical gutta-percha seal and an 11 mm post space. The teeth were mounted in acrylic resin with 12 mm of the tooth measured from the root tip embedded in the resin and the coronal 3 mm exposed above the resin block. All specimens were labeled and randomly assigned to 3 groups of 10 (Random Allocation Software 2.0). Each group represented a different restorative option: CPC (ParaPost XP-Lab), TPC (ParaPost XH), FPC (D.T. Light-Post) (Fig. 1). The mesiodistal (MD) and faciolingual (FL) dimensions of the teeth were measured coronally with a digital caliper (700-126; Mitutoyo). The mean MD, FL, and MD×FL of each group were calculated. The variances among the groups were homogenous (Levene test: pMD=.374, pFL=.208, pMD×FL=.128). One-way ANOVA showed that the groups did not differ signiﬁcantly regarding their dimensions (FMD[2,27] =1.020/p=.374, FFL[2,27]=1.663/p=.208, FMD×FL[2,27] =2.224/p=.128) and were considered dimensionally not different. The preparation of the specimens for each group was as follows. Group CPC The post space was prepared to a size 5 (ParaPost; Coltène/Whaledent). A 4 mm long, 0.6 mm deep Maroulakos et al
antirotation groove was made at the lingual aspect of the root canal with a tungsten carbide bur (no. 170; Brasseler). A circumferential 45-degree internal bevel was created at the axial angle of the root canal wall coronally with the same bur. The root canal was rinsed with chlorhexidine gluconate 0.12% (Peridex; 3M ESPE). A post and core pattern was made with a plastic pattern (ParaPost XP-Lab; Coltène/Whaledent) and chemically initiated acrylic resin (Pattern Resin LS; GC America). The pattern was invested (PowerCast; Whip Mix Corp) and cast in Type IV gold alloy (Ney-Oro 60; Dentsply Intl) with a centrifugal casting machine. The post was airborne-particle abraded (50 mm aluminum oxide particles, 400 kPa for 2 s/cm2 to a matte ﬁnish), water steamed, and air dried. Metal primer was applied according to manufacturer guidelines (Alloy Primer; Kuraray Noritake Dental Inc). The root canal was dried with paper cones. ED primer liquids A and B (Kuraray Noritake Dental Inc) were mixed at a 1:1 ratio for 4 seconds, applied into the canal with a thin brush, left for 60 seconds, and blown with a gentle stream of air to evaporate the volatiles. One full turn of Panavia 21 catalyst and of universal paste (Kuraray Noritake Dental Inc) were mixed for 20 seconds. A thick and even layer was applied on the post, which was seated with ﬁnger pressure for 60 seconds. Cement excess was removed with a brush. Glycerol gel (Oxyguard II; Kuraray Noritake Dental Inc) was applied for 3 minutes to prevent the formation of an oxygen-inhibited polymerization zone and then removed with air-water spray. Group TPC The procedure described for CPC regarding post/canal treatment and post cementation was followed. However, no antirotation groove was created. For the core, the dentin and post were etched with 34% phosphoric acid gel (Dentsply Intl) for 15 seconds. The etchant was rinsed with air-water spray for 10 seconds. Excess moisture was removed until there was no water pooling and the tooth surface was left slightly moist. Prime&Bond NT adhesive (Dentsply Intl) was mixed with the autopolymerized activator for 2 seconds (ratio 1:1), applied on the tooth and post, and left for 20 seconds. Excess solvent was removed by air-drying for 10 seconds, beginning 10 cm away from the specimen and gradually closing to 1 cm. The air-dried surface remained glossy and not desiccated. The adhesive was light polymerized for 10 seconds (Demi Plus; Kerr Corp). Equal quantities of the core paste and catalyst were mixed for 30 seconds (Fluorocore Blue; Dentsply Intl). The mix was placed in a clear form (Paracore; Coltène/Whaledent), seated on the tooth, light polymerized for 40 seconds, and left for an additional 7 minutes of autopolymerization. Finally, the form was removed and light polymerized for another 40 seconds. Maroulakos et al
Group FPC The post space was prepared to a size 1 (DT-Light Post; Bisco Inc). The procedure described for CPC regarding root canal treatment and post cementation was followed. However, no antirotation groove was created, and the post surface was left untreated. The procedure described above for TPC regarding core fabrication was followed for FPC. Crown fabrication and cementation All cores were prepared 6 mm incisal to the ﬁnish line facially and 3 mm incisal to the ﬁnish line lingually, simulating a central incisor preparation with no remaining tooth structure above the ﬁnish line. The ﬁnish line was a 1-mm wide circumferential shoulder 3 mm coronal to the resin block with a ﬂat end, medium grit, tapered diamond (847/018; Brasseler). Crown wax patterns were made directly on the specimens with a polyvinyl siloxane putty index (Lab Putty; Coltène/ Whaledent), simulating the anatomy of an 11 mm tall central incisor, and had a lingual notch 3 mm apical to the incisal edge. They were invested and cast in Type IV gold alloy (Ney-Oro 60; Dentsply Intl). All crowns were treated and cemented as for group CPC with Panavia 21. However, the ED primer was applied only on the margin for CPC, whereas for TPC and FPC it was applied on both the tooth margin and core following the manufacturer’s guidelines. Cement excess was removed with a brush. Glycerol gel was then applied for 3 minutes and removed with air-water spray. The materials used are listed in Table 1. Figure 2 illustrates the dimensions of the post, core, and crown for each group. Aging and testing procedures All specimens were stored in saline for 1 week before testing. Two specimens per group were randomly selected to obtain micro-computed tomographic (mCT) imaging in order to detect microcracks that could have occurred as a result of root canal treatment, post space preparation, or post cementation. The 6 specimens were scanned (m-CT35; Scanco Medical AG) at 10 mm voxel size isotropic resolution (E=70 kVp, I=114 mA, 1 000 projections over a total rotation of 180 degrees, integration time 800 ms). Each scan was programmed to include the root of the specimens, resulting in 1 500 slices (15 mm) and 3.5 hours of scanning time. All specimens were thermocycled by immersion in 2 water tanks (cold, warm) with temperatures of 5 C and 55 C (16 seconds cold, 16 seconds warm, 4 seconds transfer) for a total of 6 000 cycles, which represents approximately 7 months of clinical service.37 A universal testing machine (MTS 858 Mini Bionix II; MTS Systems) was used to cyclically load the specimens at a 135-degree angle to their long axis12 with a 0 to 50 N load applied at the lingual notch at a frequency of 2 Hz for a total of 50 000 cycles, which THE JOURNAL OF PROSTHETIC DENTISTRY
Table 1. Materials used Product Parapost XP-Lab (CPC)
Parallel sided, size 5, 1.22 mm diameter
Plastic burn-out patterns
Parapost XH (TPC)
Parallel sided, size 5, 1.22 mm diameter
D.T. Light-Post (FPC)
Tapered, size 1, 1.50 mm diameter
Quartz ﬁbers bound in epoxy matrix
Pattern Resin LS
Powder: polymethylmethacrylate, polymethylmethacrylate, dibenzoyl peroxide Liquid: methylmethacrylate, 2-hydroxyethyl-methacrylate
Paste: 10-methacryloyloxydecyl dihydrogen phosphate, hydrophobic aromatic dimethacrylate, hydrophobic aliphatic dimethacrylate, silanated silica ﬁller ED primer: 2-hydroxyethyl methacrylate, 10-methacryloyloxydecyl dihydrogen phosphate, N-methacryloyl-5-aminosalicylic acid Oxyguard II: glycerol, polyethylene glycol
Kuraray Noritake Dental Inc
6-(4-Vinylbenzyl-N-propyl)amino-1,3,5-triazine-2,4 dithione, 10-MDP
Kuraray Noritake Dental Inc
Prime & Bond NT Dual Cure
Prime and bond NT: urethane dimethacrylate resin, dipentaerythritol pentaacrylate phosphate, polymerizable dimethacrylate/ trimethacrylate resins, acetone Self-cure activator: acetone, urethane dimethacrylate monomer, 2-hydroxyethyl methacrylate, diphenyl(2, 4, 6-trimethylbenzoyl)phosphine Caulk 34% tooth conditioner gel: Phosphoric acid
Barium ﬂuoroaluminoborosilicate glass, treated hydrophobic fumed silica, urethane dimethacrylate resin, urethane modiﬁed bis-GMA dimethacrylate resin, polymerizable dimethacrylate/trimethacrylate resin
Au 56.0, Pd 4.0, Ag 19.9, Cu 17.0, Zn/Ir trace
5 mm 6 mm 3 mm 8 mm 4 mm CPC
Figure 2. Schematic dimensions of post, core, and crown for each group. CPC, custom gold cast post and core; TPC, prefabricated titanium post/ composite resin core; FPC, prefabricated quartz ﬁber reinforced post/ composite resin core.
reﬂects approximately 3 to 12 months of clinical service (Fig. 3).38 The 6 specimens that were evaluated with mCT before fatigue were rescanned to evaluate failure tendencies. Finally, clinical failure was induced with a universal testing machine (model 5567; Instron) with a load cell of maximum capacity of 1 000 N. The compressive force was applied at 135 degrees to the long axis at the lingual notch with a crosshead speed of 0.5 cm/min.12 The force applied to the specimen over time was recorded. Failure was deﬁned as the load recorded when the force-time graph showed a sudden drop, indicating a sudden decrease of the specimen’s resistance to compressive stress. THE JOURNAL OF PROSTHETIC DENTISTRY
Figure 3. Specimen conﬁguration for load test on universal testing machine.
Sample size was calculated with 80% power to detect differences among groups at a=.05 using statistical software (G*Power 220.127.116.11; Erdfelder, Faul & Buchner). The mean failure values for each group were calculated in newtons. The normality of distribution in each group was tested with the Shapiro-Wilk test. The homogeneity of variances among the groups was tested with the Levene test. One-way ANOVA was used to identify differences within and between the groups using “load” as a dependent variable (a=.05), and post hoc tests (Bonferroni correction) were used to locate differences (SPSS v19.0; IBM Corp). In addition, the specimens were Maroulakos et al
Table 2. Descriptive statistics for each group
Table 3. Inferential statistical results
Fracture Resistance (N)
Total Post hoc Bonferroni
Normal distribution in every group was veriﬁed with Shapiro-Wilk test (P>.05). Homogeneity of variances among groups was veriﬁed with Levene test (P>.05).
observed under the light microscope to characterize failures. The failures were classiﬁed as follows: failure of the crown (crown fracture, Type 1), the crown-core interface (crown debonding, Type 2), the post (post fracture, Type 3), the post-dentin interface (post debonding Type, 4), or the dentin (root fracture, Type 5). RESULTS The mean (SD) failure value of CPC was 174.0 N (51.0), of TPC 123.5 N (23.4), and of FPC 117.6 N (19.3) (Table 2). One-way ANOVA showed statistically significant differences among the groups [F(2,27)=8.197, P=.002]. The fracture resistance of CPC was higher than either TPC (P=.008) or FPC (P=.003). The fracture resistance of TPC was not signiﬁcantly different than FPC (P=1.000) (Table 3). Evaluation of the mCT images taken before and after aging of the 6 selected teeth led to the following observations. The best-quality images were obtained with the specimens restored with ﬁber or titanium prefabricated post/composite resin core. The specimens restored with a custom cast post and core showed a great amount of scatter that made evaluation difﬁcult. The before-aging scans showed an absence of microcracks in the radicular dentin. However, voids between the post and the radicular dentin were evident in many slices along the root of the evaluated specimens. Microgaps were evident within the body of the ﬁber posts. The after-aging scans were not remarkably different from the before-aging scans (Fig. 4). The primary mode of failure for CPC was root fracture (Type 5). In 2 specimens, the post was debonded, and in 1 the post was fractured (Type 3). For TPC, all specimens but 1 failed by root fracture (Type 5), while in 1 the post was debonded. Finally, for FPC, the primary mode of failure was post debonding (Type 4), while 3 of the specimens failed by root fracture (Fig. 5). In all cases of root fracture, the fracture line was located on the mesial or distal aspect of the root. In the cases of post debonding, for CPC and TPC, remnants of the cement could be seen on the post surface, while for FPC no cement was noticed on the post surface after post debonding. None of the groups exhibited failure of the core/crown interface. Maroulakos et al
Sum of Squares
Differences between mean values with same superscript were signiﬁcantly different (P.05).
DISCUSSION This study showed that group CPC performed better than TPC and FPC. The results support the rejection of the null hypothesis that the fracture resistance of the 3 groups would not be statistically different. In addition, modes of failure were different among the groups. Previous studies that compared different posts show various and sometimes confusing results. An in vitro study17 comparing the fracture resistance of adhesively cemented titanium, prefabricated, glass ﬁber, and carbon ﬁber posts on teeth with 2 mm of remaining tooth structure favored titanium posts. However, the teeth were not restored with crowns, negating the ferrule effect. Another compared metallic with nonmetallic posts cemented with adhesive or nonadhesive cements on teeth with 2 mm of remaining tooth structure.18 The authors concluded that ﬁber posts showed greater fracture resistance than cast post and cores and that the use of resin cement did not improve the performance of metallic posts. Other studies using static loads favored cast and titanium prefabricated over ﬁber posts,14 cast over ﬁber,16 cast and ﬁber over titanium and stainless steel,19 or prefabricated ﬁber and titanium over custom zirconia and cast posts.20 The fracture resistance rates varied from 300 to 600 N or higher,17-20 rates signiﬁcantly higher than the ones observed in this study. This may be attributed to the various levels of remaining tooth structure used, whereas in our study there was no remaining tooth structure. However, in a study in which similar materials and failure protocol were used to compare titanium prefabricated and quartz ﬁber posts, the values of fracture resistance of the studied groups were as high as in the previous studies, approximately 500 N.23 Similarly, in this current study, these groups showed similar fracture resistance but at much lower fracture values, possibly caused by the combination of cyclic loading and thermal fatigue that was not present in the previous study. Another study, in which the same post systems were used (ParaPost XP and Parapost XH) in teeth with 1 mm of remaining tooth structure, showed more comparable results, 207.3 (13.5) N for the cast post and core group and 284.7 (16.4) N for the titanium prefabricated post group.14 However, the post surface was THE JOURNAL OF PROSTHETIC DENTISTRY
Figure 4. Inverted mCT images of representative specimens. A, Custom gold cast post before aging. B, Custom gold cast post after aging. C, Titanium prefabricated post before aging. D, Titanium prefabricated post after aging. E, Quartz ﬁber reinforced post before aging. F, Quartz ﬁber reinforced post after aging. Single black arrows ([), cement voids; double black arrows ([[), microgaps in ﬁber posts.
not treated, and no artiﬁcial aging was performed. A study comparing adhesively cemented zirconia, glass ﬁber, stainless steel, and cast posts did not show any statistical difference among the groups, but the zirconia posts showed the lowest number of load cycles to failure and metal posts the highest.22 The amount of remaining tooth structure was not reported, and whether crowns were fabricated was not speciﬁed. Other studies using dynamic loading favored ﬁber over metal prefabricated21 and cast over ﬁber posts.15 THE JOURNAL OF PROSTHETIC DENTISTRY
In the present study, group CPC showed signiﬁcantly higher fracture resistance compared with FPC. This may be attributed to better adaptation of the cast posts or better bond to resin cements, especially when they are treated with primers.35 Also, the double tapered design and absence of serrations in the ﬁber posts may have reduced their mechanical retention. Previous research suggests that altering the surface of ﬁber posts can improve the bond to resin. Several materials have been used;28-30 however, there is no consensus that one Maroulakos et al
80% 70% 60% 50% 40% 30% 20% 10% 0%
Group Type 1 (0% frequency) Type 3 Type 4
Type 2 (0% frequency) Type 5
Figure 5. Frequency rate of failure modes observed for each group. Type 1, crown fracture; Type 2, crown debonding; Type 3, post fracture; Type 4, post debonding; Type 5, root fracture; CPC, custom gold cast post and core; TPC, prefabricated titanium post/composite resin core; FPC, prefabricated quartz ﬁber reinforced post/composite resin core.
material is better, and most manufacturers do not recommend altering the surface of ﬁber posts. Also, the effect of airborne-particle abrasion on ﬁber post morphologic characteristics and properties is not well deﬁned and cannot be applied safely to all systems.31 The poorer bond quality was also veriﬁed by the main failure mode, post debonding, and the absence of adhered cement on the debonded ﬁber posts. This was in agreement with existing data supporting post debonding as the major failure pattern of ﬁber posts and less frequent root fracture.32,33 Group CPC showed greater fracture resistance compared with TPC. TPC exhibited the highest rate of root fracture at signiﬁcantly lower force. The higher modulus of elasticity of titanium posts compared with posts made of gold alloys, ﬁber posts, and dentin36 may have resulted in higher stresses being transferred to dentin during loading. To evaluate the clinical signiﬁcance of these ﬁndings, the results should be compared with reported maximum occlusal forces on anterior teeth. In one study, the mean maximum anterior tooth occlusal force was 200 to 228 N.39 Another study reported a mean maximum incisor occlusal force of 93 to 150N for a white and 140 to 206 N for an indigenous Brazilian population.40 On the basis of these ﬁndings, 180 to 200 N of fracture resistance can be considered a safe evaluation threshold. Among the groups, only CPC, with a mean of 174 N, approaches this threshold. This is in agreement with the clinical guideline for using custom cast post and cores in structurally compromised teeth.3 Using teeth with no remaining tooth structure allowed a direct comparison among the post systems without the inﬂuence of the ferrule effect. This allowed direct load transfer to the root, and despite being previously used for compromised teeth,23 it may be a limitation of the study. Maroulakos et al
Also, a gentle air stream was used to evaporate the volatiles of the ED primer, as indicated by the manufacturer. However, other studies have shown an improved bond strength when paper points,42 paper points with airdrying,43 or intracanal air-drying are used to remove the solvent and excess adhesive.44 The resin cement was applied only on the post, which may have resulted in the observed cement voids. The use of a rotary spiral paste ﬁller reduces that possibility,34 but it is contraindicated by the manufacturer. Another potential limitation was the fact that clinical failure was used to determine when the specimens failed. However, it is uncommon that posts fail after a single catastrophic force. Preliminary failure occurs as a result of micromovement of the crown margin in relation to the tooth. This occurs much earlier than clinically visible failure and is not as easily detected.7 This can be particularly important in the case of bonded posts, because when clinical failure occurs, it may lead to an eventually nonrestorable tooth. The low fracture resistance rates in our study could be partly explained by the aging-induced degradation of the adhesive interfaces (storage in water, thermocycling and cyclic loading fatigue). Finally, the results of this study may be directly related to the materials/ methodology used and may not reﬂect what would happen under different conditions. The resin cement used was allowed to set at room temperature (23 C), which is lower than body temperature. As shown with other adhesive cements, the degree of polymerization, polymerization shrinkage, and reaction kinetics and timing may have been affected by the experimental conditions.45,46 The failure loading protocol did not include a dynamic approach that could reproduce the oral conditions more closely. Future studies should compare groups with different levels of less than ideal tooth structure by using an accelerated fatigue protocol to explore the inﬂuence of the interaction between post type and remaining tooth structure on the fatigue resistance of endodontically treated teeth. CONCLUSIONS Within the limitations of this in vitro study, the following conclusions were drawn: 1. The type of post and core system signiﬁcantly inﬂuences the fracture resistance of structurally compromised endodontically treated teeth. The bonded gold cast post and core showed higher fracture resistance than the other systems tested. 2. Teeth restored with quartz ﬁber posts exhibit more favorable failure patterns but at a very low fracture resistance value. REFERENCES 1. Isidor F, Brondum K, Ravnholt G. The inﬂuence of post length and crown ferrule length on the resistance to cyclic loading of bovine teeth with prefabricated titanium posts. Int J Prosthodont 1999;12:78-82.
THE JOURNAL OF PROSTHETIC DENTISTRY
2. Giovani AR, Vansan LP, de Sousa Neto MD, Paulino SM. In vitro fracture resistance of glass-ﬁber and cast metal posts with different lengths. J Prosthet Dent 2009;101:183-8. 3. Torbjorner A, Fransson B. A literature review on the prosthetic treatment of structurally compromised teeth. Int J Prosthodont 2004;17:369-76. 4. Gegauff AG. Effect of crown lengthening and ferrule placement on static load failure of cemented cast post-cores and crowns. J Prosthet Dent 2000;84: 169-79. 5. The glossary of prosthodontic terms. J Prosthet Dent 2005;94:10-92. 6. Sorensen JA, Engelman MJ. Ferrule design and fracture resistance of endodontically treated teeth. J Prosthet Dent 1990;63:529-36. 7. Libman WJ, Nicholls JI. Load fatigue of teeth restored with cast posts and cores and complete crowns. Int J Prosthodont 1995;8:155-61. 8. Ng CC, al-Bayat MI, Dumbrigue HB, Griggs JA, Wakeﬁeld CW. Effect of no ferrule on failure of teeth restored with bonded posts and cores. Gen Dent 2004;52:143-6. 9. Milot P, Stein RS. Root fracture in endodontically treated teeth related to post selection and crown design. J Prosthet Dent 1992;68:428-35. 10. Assif D, Oren E, Marshak BL, Aviv I. Photoelastic analysis of stress transfer by endodontically treated teeth to the supporting structure using different restorative techniques. J Prosthet Dent 1989;61:535-43. 11. Tan PL, Aquilino SA, Gratton DG, Stanford CM, Tan SC, Johnson WT, et al. In vitro fracture resistance of endodontically treated central incisors with varying ferrule heights and conﬁgurations. J Prosthet Dent 2005;93:331-6. 12. Ng CC, Dumbrigue HB, Al-Bayat MI, Griggs JA, Wakeﬁeld CW. Inﬂuence of remaining coronal tooth structure location on the fracture resistance of restored endodontically treated anterior teeth. J Prosthet Dent 2006;95:290-6. 13. Goto Y, Swift EJ Jr. Ferrules for endodontically treated teeth. J Esthet Restor Dent 2009;21:292-3. 14. Cormier CJ, Burns DR, Moon P. In vitro comparison of the fracture resistance and failure mode of ﬁber, ceramic, and conventional post systems at various stages of restoration. J Prosthodont 2001;10:26-36. 15. Sahaﬁ A, Peutzfeldt A, Ravnholt G, Asmussen E, Gotfredsen K. Resistance to cyclic loading of teeth restored with posts. Clin Oral Investig 2005;9:84-90. 16. Varvara G, Perinetti G, Di Iorio D, Murmura G, Caputi S. In vitro evaluation of fracture resistance and failure mode of internally restored endodontically treated maxillary incisors with differing heights of residual dentin. J Prosthet Dent 2007;98:365-72. 17. Al-Wahadni AM, Hamdan S, Al-Omiri M, Hammad MM, Hatamleh MM. Fracture resistance of teeth restored with different post systems: in vitro study. Oral Surg Oral Med Oral Pathol Oral Radiol Endod 2008;106:e77-83. 18. Gu XH, Kern M. Fracture resistance of crowned incisors with different post systems and luting agents. J Oral Rehabil 2006;33:918-23. 19. Akkayan B, Gulmez T. Resistance to fracture of endodontically treated teeth restored with different post systems. J Prosthet Dent 2002;87:431-7. 20. Bittner N, Hill T, Randi A. Evaluation of a one-piece milled zirconia post and core with different post-and-core systems: an in vitro study. J Prosthet Dent 2010;103:369-79. 21. Goto Y, Nicholls JI, Phillips KM, Junge T. Fatigue resistance of endodontically treated teeth restored with three dowel-and-core systems. J Prosthet Dent 2005;93:45-50. 22. Jung SH, Min KS, Chang HS, Park SD, Kwon SN, Bae JM. Microleakage and fracture patterns of teeth restored with different posts under dynamic loading. J Prosthet Dent 2007;98:270-6. 23. Ayad MF, Bahannan SA, Rosenstiel SF. Inﬂuence of irrigant, dowel type, and root-reinforcing material on fracture resistance of thin-walled endodontically treated teeth. J Prosthodont 2011;20:180-9. 24. Junge T, Nicholls JI, Phillips KM, Libman WJ. Load fatigue of compromised teeth: a comparison of 3 luting cements. Int J Prosthodont 1998;11:558-64. 25. Bolhuis P, de Gee A, Feilzer A. The inﬂuence of fatigue loading on the quality of the cement layer and retention strength of carbon ﬁber post-resin composite core restorations. Oper Dent 2005;30:220-7. 26. Dietschi D, Duc O, Krejci I, Sadan A. Biomechanical considerations for the restoration of endodontically treated teeth: a systematic review of the literature, part II (Evaluation of fatigue behavior, interfaces, and in vivo studies). Quintessence Int 2008;39:117-29. 27. Naumann M, Sterzenbach G, Rosentritt M, Beuer F, Frankenberger R. Is adhesive cementation of endodontic posts necessary? J Endod 2008;34: 1006-10. 28. Schmage P, Cakir FY, Nergiz I, Pfeiffer P. Effect of surface conditioning on the retentive bond strengths of ﬁberreinforced composite posts. J Prosthet Dent 2009;102:368-77.
THE JOURNAL OF PROSTHETIC DENTISTRY
29. Yenisey M, Kulunk S. Effects of chemical surface treatments of quartz and glass ﬁber posts on the retention of a composite resin. J Prosthet Dent 2008;99:38-45. 30. Albashaireh ZS, Ghazal M, Kern M. Effects of endodontic post surface treatment, dentin conditioning, and artiﬁcial aging on the retention of glass ﬁber-reinforced composite resin posts. J Prosthet Dent 2010;103:31-9. 31. Choi Y, Pae A, Park EJ, Wright RF. The effect of surface treatment of ﬁberreinforced posts on adhesion of a resin-based luting agent. J Prosthet Dent 2010;103:362-8. 32. Rasimick BJ, Wan J, Musikant BL, Deutsch AS. A review of failure modes in teeth restored with adhesively luted endodontic dowels. J Prosthodont 2010;19:639-46. 33. Santos AF, Meira JB, Tanaka CB, Xavier TA, Ballester RY, Lima RG, et al. Can ﬁber posts increase root stresses and reduce fracture? J Dent Res 2010;89: 587-91. 34. Akgungor G, Akkayan B. Inﬂuence of dentin bonding agents and polymerization modes on the bond strength between translucent ﬁber posts and three dentin regions within a post space. J Prosthet Dent 2006;95: 368-78. 35. Yanagida H, Tanoue N, Ide T, Matsumura H. Evaluation of two dualfunctional primers and a tribochemical surface modiﬁcation system applied to the bonding of an indirect composite resin to metals. Odontology 2009;97: 103-8. 36. Plotino G, Grande NM, Bedini R, Pameijer CH, Somma F. Flexural properties of endodontic posts and human root dentin. Dent Mater 2007;23: 1129-35. 37. Amaral FL, Colucci V, Palma-Dibb RG, Corona SA. Assessment of in vitro methods used to promote adhesive interface degradation: a critical review. J Esthet Restor Dent 2007;19:340-53. 38. Wiskott HW, Nicholls JI, Belser UC. Stress fatigue: basic principles and prosthodontic implications. Int J Prosthodont 1995;8:105-16. 39. Laurell L, Lundgren D. A standardized programme for studying the occlusal force pattern during chewing and biting in prosthetically restored dentitions. J Oral Rehabil 1984;11:39-44. 40. Regalo SC, Santos CM, Vitti M, Regalo CA, de Vasconcelos PB, Mestriner W Jr, et al. Evaluation of molar and incisor bite force in indigenous compared with white population in Brazil. Arch Oral Biol 2008;53:282-6. 41. Hargreaves KM, Cohen S. Cohen’s pathways of the pulp. 10th ed. St Louis: Mosby; 2011:322-3. 42. Souza RO, Lombardo GH, Michida SM, Galhano G, Bottino MA, Valandro LF. Inﬂuence of brush type as a carrier of adhesive solutions and paper points as an adhesive-excess remover on the resin bond to root dentin. J Adhes Dent 2007;9:521-6. 43. Thitthaweerat S, Nakajima M, Foxton RM, Tagami J. Effect of solvent evaporation strategies on regional bond strength of one-step self-etch adhesives to root canal dentine. Int Endod J 2013;46:1023-31. 44. Aziz TM, Anwar MN, El-Askary FS. Push-out bond strength of ﬁber posts to root canal dentin using a one-step self-etching adhesive: the effect of solvent removal and light-curing methods. J Adhes Dent 2014;16:79-86. 45. Kitzmuller K, Graf A, Watts D, Schedle A. Setting kinetics and shrinkage of self-adhesive resin cements depend on cure-mode and temperature. Dent Mater 2011;27:544-51. 46. Oliveira M, Cesar PF, Giannini M, Rueggeberg FA, Rodrigues J, Arrais CA. Effect of temperature on the degree of conversion and working time of dualcured resin cements exposed to different curing conditions. Oper Dent 2012;37:370-9. Corresponding author: Dr Georgios Maroulakos 415 E Vine St, #304 Milwaukee, WI 53212 Email: [email protected]
Acknowledgments The authors thank Dr Jorge Jaramillo Otero, international fellow at the Department of Endodontics, Texas A&M University, Baylor College of Dentistry, for performing the endodontic treatment to the specimens. Also, thanks to Lilly Guo, research associate at the Department of Biomaterials, for her help executing the experiments with the Instron and MTS machines. Copyright © 2015 by the Editorial Council for The Journal of Prosthetic Dentistry.
Maroulakos et al